1 / 31

310 likes | 425 Vues

Engineering Diffraction: Update and Future Plans. Ersan Üstündag Iowa State University. Engineering Diffraction: Scope. Main objective : Predict lifetime and performance Needed: Accurate in-situ constitutive laws: = f() Measurement of service conditions: residual and internal stress.

Télécharger la présentation
## Engineering Diffraction: Update and Future Plans

**An Image/Link below is provided (as is) to download presentation**
Download Policy: Content on the Website is provided to you AS IS for your information and personal use and may not be sold / licensed / shared on other websites without getting consent from its author.
Content is provided to you AS IS for your information and personal use only.
Download presentation by click this link.
While downloading, if for some reason you are not able to download a presentation, the publisher may have deleted the file from their server.
During download, if you can't get a presentation, the file might be deleted by the publisher.

E N D

**Engineering Diffraction:Update and Future Plans**Ersan Üstündag Iowa State University**Engineering Diffraction: Scope**• Main objective: Predict lifetime and performance • Needed: • Accurate in-situ constitutive laws: = f() • Measurement of service conditions: residual and internal stress**Incident**h1k1l1 Scattered h1k1l1 Incident h2k2l2 Scattered h2k2l2 Engineering Diffraction: Typical Experiment Eng. Diffractometers: SMARTS (LANSCE) ENGIN X (ISIS) VULCAN (SNS) Typical engineering studies: • Deformation studies • Residual stress mapping • Texture analysis • Phase transformations Challenges: • Small strains (~0.1%) • Quick and accurate setup • Efficient experiment design and execution • Realistic pattern simulation • Real time data analysis • Realistic error propagation • Comparison to mechanics models • Microstructure simulation Bragg’s law: = 2dsin**Engineering Diffraction: Vision for DANSE**• Objectives: • Enable new science (& enhance the value of EngND output) • Utilize beam time more efficiently • Help enlarge user community • Approach: • Experiment planning and setup: (Task 7.1) • Experiment design • Optimum sample handling (SScanSS) • Error analysis • Mechanics modeling (FEA, SCM): (Task 7.2) • Multiscale (continuum to mesoscale) • Constitutive laws: = f() • Experiment simulation: (Task 7.3) • Instrument simulation (pyre-mcstas) • Microstructure simulation (forward / inverse analysis) • Impact: • Re-definition of diffraction stress analysis • Easy transfer to synchrotron XRD**Engineering Diffraction: Typical Experiment**• Proposed Applications • Experiment Design and Simulation • Instrument simulation • Optimization of parameters • Microstructure simulation • Mechanics modeling I: finite element analysis (FEA) • Mechanics modeling II: self-consistent modeling (SCM) • Data analysis Efforts underway in all of these tasks**Experiment Design and Simulation**• Instrument simulation • McStas • Machine studies (SMARTS, ENGIN X) • Optimization of parameters • Sample setup and alignment (SScanSS) • Parametric studies (e.g., neural network analysis) • Microstructure simulation • Defining the sample kernel for experiment simulation • Full forward simulation of experiment**ISIS: SScanSS Software**• Implemented on ENGIN X • Ideal for efficient sample setup • Controlled by IDL scripts • Generates a computer image of sample • Creates and executes a measurement plan • Performs GSAS analysis • Creates 2-D data/result plots J. James et al.**Experiment Design and Simulation**• Instrument characterization (machine studies) SMARTS ENGIN-X**(a)**Engineering Diffraction: Microstructure • Si single crystals (0.7 and 20 mm thick) • SMARTS data • Double peaks due to dynamical diffraction**(b)**Engineering Diffraction: Microstructure • Si single crystal (20 mm thick) • ENGIN-X depth scan • Data originates from surface layers Critical question: Transition between a single crystal and polycrystal? E. Ustundag et al., Appl. Phys. Lett. (2006)**Object Oriented Finite Element Analysis**A. Reid (NIST) • Modeling of real microstructure • Will be employed in DANSE for microstructure modeling • Needs to become 3-D and validated**[111]**[001] [111] 0.1 μm 1 μm 5 μm x-dim 5 μm z y x Three Grain Model Description Microstructure Simulation • Unixaxial Tension: σapplied = 100, 200 & 300 MPa (along x) • x-dim varies:5 μm, 3 μm, 1 μm, 0.8 μm, 0.6 μm • Cu parametersC11111 = 220.3 GPa, C11112 = 104.1 GPa, C11144 = 40.8 GPa C00111 = 168.4 GPa, C00112 = 121.4 GPa, C00144 = 75.4 GPa I.C. Noyan et al.**0.1 μm**1 μm Bulk Strain Values Interaction strain we are interested in measuring. 5 μm 3 μm 5 μm z y x Results from FE Model (300 MPa) • Using COMSOL Multiphysics, we obtain the out of plane strain along center line in central grain. I.C. Noyan et al.**~0.05o**Individual Peaks Kinematic X-Ray Modeling • Using kinematic diffraction theory, we simulate a rocking curve diffraction pattern. • Total peak shift of ~0.05o from any one edge. I.C. Noyan et al.**Peak Fitting Analysis**• Fitting the diffraction peak with multiple Gaussians, it is possible to determine the peak position and breadth at each step of the summation. • A FWHM value does not necessarily predict a unique strain distribution in a specimen. • How to determine strain profiles from peak position and shape? • What happens in the inelastic regime? I.C. Noyan et al.**Mechanics Modeling**• Finite element analysis (FEA) • ABAQUS • Optimization of material parameters • Self-consistent modeling (SCM) • EPSC code from LANL • Optimization of material parameters**Mechanics Modeling:FEA (Finite Element Analysis)**Laptop SNS Linux cluster (P) NeXus Archive E1, Y1, E2, Y2 Rietveld ABAQUS a1(P), a2(P) 1c, 2c 1(a1), 2(a2) Compare (fmin) & Optimize (E1,Y1…) 1(1), 2(2)**Framework**Optimizer ABAQUS CALL Visualizer call services call services Preprocessor Main processor Postprocessor Use Case Diagram for FEA Application**BMG**W-BMG composite Example: BMG-W fiber composite • Residual stresses • Compression loading at SMARTS • Experiments on 20% to 80% volume fraction of W • Unit cell finite element model • GSAS output for average elastic strain in W in the longitudinal direction 20% W/BMG 80% W/BMG Reference: B. Clausen et al., Scripta Mater. 49 (2003) p. 123**Voce**Power-law Activity Diagram: FEA (Finite Element Analysis) (P) <include> E1, Y1, E2, Y2 <include> ABAQUS experimental data 1c, 2c 1(a1), 2(a2) Compare & Optimize <include> <include> leastsq fmin 1(1), 2(2) Easy utilization of various software components**σ**σ θ0 θ1 n=1 n=4 σo σo n=∞ εo ε εo ε Constitutive Laws for W and BMG Voce Power-law σ1 W BMG Input parameters: (σ0)BMG, nBMG, (σ0)W, (σ1)W, (θ0)W, (θ1)Wand T**Neural Network Analysis**Sensitivity Studies • Strong influence by parameters: (σ0)BMG, (σ0)W, (σ1)W and (θ0)W • Weak/no influence by parameters: nBMG,(θ1)W and T • Rigorous experiment planning to optimize data collection L. Li et al.**Neural Network Analysis**Result • Use of experimental data for inverse analysis • Prediction of ‘optimum’ values of all 7 input parameters • Previous analyses optimized only 3 parameters L. Li et al.**FEA (Finite Element Analysis)**Custom (standard) geometries as templates API release planned for 2007**Mechanics Modeling: Self-Consistent Model**<include> Reduce NeXus file User <include> EPSC () • In collaboration with C. Tome (LANL) • Parallel modularization of EPSC, VPSC codes and DANSE implementation <include> I(TOF) pyre-mcstas • Self-consistent modeling (SCM) • Estimate of lattice strain (hkl dependent) • Study of deformation mechanisms**Data Analysis**• Peak fitting • Rietveld (full-pattern) analysis GSAS, DiffLab • Single peak fitting • Integration of mechanics models to peak fitting • Strain anisotropy analysis • Texture analysis and visualization (MAUD) • Real-time data analysis**Data Analysis: Mechanical Loading of BaTiO3**• Time-of-flight neutron diffraction data from ISIS • Complete diffraction patterns in one setting • Simultaneous measurement of two strain directions • Different data analysis approaches: • Single peak fitting: natural candidate; but some peaks vanish as the corresponding domain is depleted • Rietveld: crystallographic model fit to all peaks; but results are ambiguous • Constrained Rietveld: multi-peak fitting, but accounting for strain anisotropy (rsca); most promising M. Motahari et al. 2006**Strain Anisotropy Analysis**• Desirable to perform multi-peak fitting (e.g. via Rietveld analysis) to improve counting statistics. • Question: How to account for strain anisotropy (hkl-dependent) due to elastic constants and inelastic deformation (e.g., domain switching)? • Current approach for cubic crystals (in GSAS): • is called ‘rsca’ and is a refined parameter for some peak profiles. • Works reasonably well in the elastic regime, but not beyond. • Needed: rigorous multi-peak fitting with peak weighting and peak shift dictated by mechanics modeling. Integration of crystallographic and mechanics models**Engineering Diffraction: Team**• E. Üstündag‡, S. Y. Lee, S. M. Motahari, G. Tutuncu (ISU) • X. L. Wang‡(SNS) - VULCAN • C. Noyan‡, L. Li, A. Ying(Columbia) – microstructure • M. Daymond‡(Queens U., ISIS) – ENGIN X, SCM • L. Edwards‡ and J. James (Open U., U.K.) - SScanSS • C. Aydiner, B. Clausen‡, D. Brown, M. Bourke(LANSCE) - SMARTS • J. Richardson‡ (IPNS) • P. Dawson (Cornell) – 3-D FEA • H. Ceylan (ISU) - optimization ‡ Member of EngND Executive Committee

More Related